Catalytic cracking of polypropylene waste over zeolite beta
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201331Catalytic Cracking of Polypropylene Waste over Zeolite BetaKatnanipa Wanchai*Aticha ChaisuwanDepartment of Chemistry, Faculty of Science, Chulalongkorn University, Bangkok, Thailand.*E-mail of corresponding author: firstname.lastname@example.orgAbstractCatalytic cracking of polypropylene (PP) waste has been investigated using zeolite beta (BEA) as a catalyst. BEAwas performed by transformation of mesoporous silica SBA-15, a novel synthesis based on the functionalization ofSi/Al ratio was studied. The catalyst samples obtained were tested for their catalytic activities in the cracking of PPwaste in batch reactor under various conditions. The plastic conversions and the yields of products fractionsobviously depend on the the Si/Al ratios and reaction temperatures. The product selectivity is affected by thosefactors. The thermal cracking of PP waste leads to plastic %conversion lower than catalytic cracking. In contrast, thenanoparticle BEA is found very active up to 95 %conversion. The used catalyst can be regenerated easily bycalcination and its activity remains comparable to the fresh catalyst.Keywords: Zeolite beta, Catalytic cracking, Thermal cracking, Polypropylene (PP) waste, %conversion1. IntroductionIn recent years, the production and consumption of plastic have increased drastically. The amount of waste plasticsgenerated from domestic and industrial usage of plastic is growing continuously. They are mostly landfilled orincinerated as conventional ways to the disposal of waste plastics. However, these methods are facing a great socialresistance due to the air pollution and soil contamination (Lee 2002). In Thailand, plastic waste from household,industrial process and market are 2.7 million ton per year and 0.2 million tons for recycling (TEENT 2012). Therecycling plastic waste method has been developed and new recycling approaches are being investigated. Thechemical recycling can lead to total depolymerization to the monomers, or partial degradation to other secondaryvaluable materials. Energy recovery is an effective way to reduce the volume of organic materials by incineration.Among the recycling techniques, the incineration meet with strong societal opposition and mechanical recycling canbe carried out only on single-polymer waste streams. However, the most effective method, in accordance with theprinciples of sustainable development, is chemical recycling also called as feedstock. According to this method,waste polymers can be either converted to original monomers or other valuable chemicals. These products are usefulas feedstock for a variety of downstream industrial processes or as transportation fuel (Scheirs 1998 and Achilias &Karayannidis 2004).Thermal cracking involves the degradation of the polymeric material with high temperature (>700oC) when it isapplied under inert atmospheric conditions. In the case of polyolefins like polyethylene, polypropylene, this processhas been reported to proceed through a random scission mechanism that generates a heterogenous mixture such aslinear parafins, olefins and aromatic compounds. At low temperature (400-500oC) the three fractions received ahigh-calorific value gas, condensable hydrocarbon oil and wax (Aguado et al. 2008 and Achilias & Megalokonomos2006). Due to the low thermal conductivity of polymer together with the endotherm of cracking, thermal pyrolysisconsumes a large amount of energy. Thus, catalytic technologies have been proposed to promote cracking at lowtemperature, resulting in reduced energy consumption and higher conversion rates (Manos et al. 2002). Catalyticcracking is most important to the shape selectivity exhibited by certain catalysts allows the formation of a narrowerdistribution of hydrocarbon products, which may be directed towards light and aromatic hydrocarbons with highermarket values (Seo et al. 2003 and Artetxe et al. 2012). Heterogeneous catalysis has been investigated extensivelyusing solids with acid properties. Several studies have been conducted describing the cracking of pure polyolefinsover different acid solids like zeolites and mesoporous material (Panda & Singh 2011, Aguado et al. 2000, Obali etal. 2012 and Aguado et al. 2000). Zeolites which are classified as a group of microporous materials are widely usedas acid catalysts, especially in the petrochemical industry due to the fact that they possess several desirableproperties such as high acidity, unique pore structure with kinetic pore size, high specific adjustable surface area andhydrophilicity, high thermal stability (Renzini et al. 2011). Zeolites of the kind employed in the catalytic crackingof hydrocarbon feedstocks such as ZSM-5, zeolite Y and zeolite beta are being the most studied (Manos et al. 2002).
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201332Cracking with acid catalysts takes place through the formation of carbocation, which requires the presence of strongacidic regions. Acid strength and textural properties are the main parameters dictating the performance of acid solidsin the catalytic conversion polymer. Porosity, surface area and particle size determine to a large extent theaccessibility of bulky polymeric molecules to the internal catalytic acid sites of solids.Zeolite beta which has a structure code of BEA established by International Zeolite Association is high silica, large-pore zeolite with a three-dimensional channel system and large 12- membered ring pore openings are the mostattractive zeolite nowadays. BEA is used as a solid acid catalyst for several industrial processes especially cracking(Renzini et al. 2011 and Nakao et al. 2004), isomerization (Kumar et al. 2007), alkylation (Bregolato et al. 2007),and oxidation (Xia & Tatsumi 2005 and Hulea & Dumitriu 2004). Though the synthesis of BEA has not widelydeveloped comparing to ZSM-5 due to the concurrence of its polymorphs, the effective synthesis can be carried outby using a particular pore directing agent, i.e. tetraethylammonium hydroxide. After extensive studies in itsapplications, the development of the synthesis of BEA becomes interesting. Zeolites are known for strong acidityand high specific surface area, but those characteristics are not enough for being excellent cracking catalysts. It wassuggested that initial polyolefin cracking occurs mainly at the acid sites on the external surface of a zeolite(Wadlinger et al. 1967). Only small enough intermediates are able to enter the zeolite pores or channels and reactwith the internal acid sites of the zeolite. The external surface area plays more important role than the internal onefor cracking of large molecules like polyolefin plastics to valuable small hydrocarbon molecules. Polyolefin wastescan be converted into petroleum feedstock, gasoline-range fuel via the cracking method (Lee et al. 2008). BEA canbe synthesized by several methods. The dry-gel method is typically conducted by separating liquid from the dry gelcompletely during the course of crystallization. During the practice, the preparation of the stiff dry gel was ratherinconvenient. The fluoride method was later developed by using the corroding reagent until the large crystal size ofBEA was obtained. The latest practical method is the xerogel method which can be regarded as a modifiedhydrothermal synthesis. The silica sources preferred in the zeolite synthesis are such as fumed silica (Aguado et al.1997), silica xerogel (Aguado et al. 2000), kanemite (Ding et al. 2006), FAU (Selvam et al. 2003) and MCM-41(Jon et al. 2006). In this study we synthesized BEA from mesoporous silica, using it as a silica source which isprepared by using non expensive templating agent (P123). Our BEA have been prepared and compared their activityin the catalytic cracking of PP waste.2. Experimental2.1 ChemicalsTetraethylorthosilicate (TEOS) and tetraethylammonium hydroxide (TEAOH) were supplied by Fluka andaluminum isopropoxide (AIP) from Merck. Pluronic P123 was purchased from Aldrich and hydrochloric was fromBDH Chemicals.2.2 CatalystsZeolite beta (BEA) used in this work was synthesized using the transformation of SBA-15 to BEA method. Thecalcined SBA-15 to be used as a silica source that prepared in acidic media using a triblock copolymer PluronicP123 as structure directing agent following a method of Zhao et al (1998). The gel with the following molarcomposition of reaction mixture was: SiO2:xAl2O3:0.26TEAOH:5.0H2O (x = 0.0055-0.049). Thereby, the mixture ofAIP and TEAOH solution was drop wise added to calcine SBA-15 with stirring. Then the mixture was aged andstirring. The gel mixture was transfered into a stainless-steel autoclave containing Teflon cup and kept in the oven at135oC for 48 h. After that white solid sample was separated by centrifugation, washed several times with deionizedwater and dried in the oven at 110oC overnight.2.3 CharacterizationThe BEA products were structurally identified using a Rigaku D/MAX-2200 Ultima-plus X-ray powder diffraction(XRD) with a monochromator for Cu Kα radiation. For the Bragg angle measurement from 5-40 deg, the divergence,scattering, and receiving slits are set at 0.5 deg, 0.5 deg, and 0.3 mm, respectively. Solid state 27Al-MAS-NMR
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201333spectra were performed using the Bruker Advance DPX 300 MHz NMR spectrometer. The material morphologywas characterized using a JEOL JSM-5410 LV scanning electron microscope (SEM). The nitrogen adsorptionisotherms were obtained using a BELSORP mini-II with 40 mg of sample. The specific surface area was analyzedusing BET plot. The external surface area and micropore volume were determined by the t-plot analysis using theadsorption branch of the isotherm. Acid strength of catalysts was determined using the BEL Japan, BELCAT withthe sample weight about 100 mg and highly pure ammonia gas as the probe molecule and helium as the auxiliary gas.2.4 Catalytic cracking experimentsDegradation of PP waste was performed using BEA catalysts with Si/Al ratio of 30, 60 and 90. Thermal andcatalytic cracking reactions were carried out in glass under a continuous nitrogen flow by batch operation. Thecracking reaction was performed at 40 min in batch reactor with a continuous nitrogen flow 20 ml/min. The effect ofcracking temperature was studied by varying from 350 to 420°C. In each experiment, 5 g of plastic were loaded intothe single reactor and mixed with an appropriate amount of calcined catalyst power (plastic/catalyst ratio of 5%w/w). The reactor was heated to the desired reaction temperature within 15 min approximately, and the temperaturewas hold for 30 min after reading the reaction temperature. Gas products were analyzed using Varian CP 3800 GCequipped with an KCl/Alumina-PLOT column (30 m x 0.35 mm), whereas liquid product obtained from the reactionwas separated into two fractions, distillate oil and heavy oil, by vacuum distillation at the heater temperature of200oC. The distillate oils were analyzed using a Varian a CP 3800 GC with CP-sil 5 column (30 m x 0.25 mm). Aflame ionization detector was utilized for all GC analysis. The values of retention time of components in thedistillate oil on a gas chromatogram were compared to those of reference compounds in the form of n-paraffins. Thevalues of %conversion and % yield were calculated based on the equations as follows:% Conversion =plasticofmass100xfraction)gasofmassfractionproductliquidof(mass +mass of gas fraction = (a – b)Where a = mass of the reactor with plastic and catalyst before reactionb = mass of the reactor with residue and used catalyst after reaction% Yield =plasticofmass100xfractionproductofmass3. Results and discussion3.1 Catalysts characterization3.1.1 Powder X-ray diffraction and Scanning electron microscopyThe XRD patterns of calcined products obtained with different Si/Al ratios are shown in Figure 1. The Si/Al ratiosof 30, 60 and 90 exhibited XRD pattern with diffraction peaks coincident with the pure phase BEA structure andhigh crystallinity can be achieved as shown in Figure 1b and 1c. With further increasing the Si/Al ratio to 90, theintensities of characteristic XRD peaks of BEA (Figure 1d) decreased. For the Si/Al ratio as low as 10, the failure offormation of BEA is depended on the amount of organic template, under the synthesis condition acting as theskeleton for inorganic ions to adhere. Obviously, it was not enough for all ions especially aluminum ionic species toform aluminosilicate building blocks. It seems that higher amount of TEAOH/Si is required for making the BEAwith low Si/Al ratio. Thus, the excess amount of aluminum turns to be located at the extra-framework octahedralposition instead of the framework tetrahedral site. This fact can be proven by 27Al-MAS-NMR spectra of productswith different Si/Al ratios in Figure 2. The spectra of calcined products show the presence of an intense signalcentered at around 55 ppm (tetrahedral framework) and small signal at about 0 ppm (octahedral framework). Theproduct at Si/Al ratios of 90 gives the signal at around 0 ppm with lower intensity than other samples. It indicatesthat the lower Si/Al ratio, the higher intensity of the peak assigned for the octahedral aluminum site is found. As a
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201334result, the Si/Al ratio of 10 is not suitable to prepare BEA by this method. In other words, the large amount of AIPwith the low Si/Al ratio can be considered as the diminishing of the uniform of tetrahedral unit in the structure ofBEA. It is obvious that the drastic decrease in crystallinity of high Si/Al ratio is not due to the effect of particle size.It indicates that the Si/Al ratio in reactant media can play an important role on the formation of the BEA structure bythis synthesis methodThe SEM image of the starting SBA-15 (Figure 3a) is different from all the rest. That is, the particle shape of SBA-15 is the rope-like bundles of rods. In the presence of TEAOH and AIP, the SBA-15 rods disintegrate apart andrecrystallize to form BEA at Si/Al ratio ranging from 30 to 90. The sample Si/Al of 10 shows large particles ofamorphous phase with some particles of remaining SBA-15 as displayed in Figure 3b. The remaining SBA-15 is inagreement with the small angle XRD results in Figure 1a. Moreover, the SEM images of BEA with various Si/Alratios are illustrated in Figure 3c to 3e. The BEA particles are fairly spherical shaped and the surface is not smooth.Additionally, the ranges of particle size are not quite different among the three samples of BEA (173-215 nm) withSi/Al ranging from 30 to 126.96.36.199 Nitrogen adsorptionThe nitrogen adsorption isotherms of calcined SBA-15 and BEA products with various Si/Al ratios are compared inFigure 4. SBA-15 exhibits a type IV adsorption isotherm which is a characteristic pattern of mesoporous material,and its BET surface area is 797 m2/g. The products synthesized using the reactant mixture containing Si/Al ratios of30 and 60 are the type I isotherms of microporous behavior. It is obvious that the Si/Al ratio of 30 provided with thesample has higher external surface area than the Si/Al ratio of 60 (Table 1). It is evident that the increase in externalsurface area is affected by the particle nano-size. The BEA product obtained from the reactant mixture with the Si/Alratio of 90 shows the hysteresis loop in the region of the relative pressure around 0.5-0.8 indicating the mesoporousbehavior along with the microporous character at the very low relative pressure. The result is in agreement with thelow crystallinity, related to the decreased order of the zeolite structure. The BET surface areas are varied in the rangebetween 455 and 782 m2/g. Besides, the samples with high crystallinity show higher BET specific surface areas, andonly the BEA sample synthesized with Si/Al of 30 in the starting mixture displays the extremely high externalsurface area.3.1.3 NH3-TPD profilesFigure 5 exhibits NH3-TPD profiles of calcined SBA-15 and transformation products with different Si/Al ratios. TheNH3 desorption peak centered at 170oC is typically assigned to a weaker acid Bronsted, or Lewis site, or even tosilanol groups. The component peak at 430oC is assigned to a stronger acid Bronsted and Lewis site. It is found thatthe peak at 170oC is more pronounced for all samples but in different extent. The acidities of the zeolite samples areconcluded in Table 1. It is noted that the total acidity of the zeolite samples is inversely proportional to the Si/Alratio used in the synthesis course. As usual, the lower the Si/Al ratio, the higher the acidity is the [AlO2]-tetrahedralunits in the zeolite framework are accounted for the acidity of the zeolite samples. It is noticeable that the results aresimilar to Sakthivel et al. (2009). The product with the Si/Al ratio of 30 shows the highest number of acid sites.3.2 Catalytic cracking of polypropylene3.2.1 The effect of Si/Al ratios and reaction temperatureThe effect of Si/Al ratios of 30, 60 and 90 was tested in catalytic cracking of PP waste at the low temperature of350°C. The low temperature was used in order to avoid the competition of thermal cracking of PP waste. The %conversion has been calculated by taking into account only the liquid and gas products that evaporated from thereactor at the reaction temperature. The results are shown in Table 2. The liquid fraction of thermal cracking is notobtained at all and the conversion of plastic is only 2.0% whereas it is in the range from 42.9 to 50.5% for catalyticcracking. The result indicates the difficulty in cracking PP waste without catalyst at low temperature. Therefore, thetotal weight loss of plastic precursor after reaction is dedicated to gas fraction. In the presence of BEA, theconversion drastically increases from 2.0% to about 42 to 50%. The results indicate that the waxy residuedecomposed into relatively lighter liquid hydrocarbons resulting in higher yield of liquid fraction than the case ofthermal cracking. The Si/Al ratio of 30 gives the highest %conversion due to the influence of zeolite external surfacearea and strong acidity, determined by NH3-TPD. The high external surface area contains the great numbers of
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201335external acid sites, which may play an important role on the cracking of bulky molecule such as polymer (Isihara etal. 1992). This fact favors long-chain polymer scission reactions, and a highly cracked product with shorterhydrocarbon chains is obtains. The synergism of catalyst surface area, external surface area and acidity of BEASi/Al of 30 contributes to the PP waste conversion in the cracking process. The profiles of gas product distributionof thermal cracking and catalytic cracking are shown in Figure 6. For thermal cracking, propene, n-pentane and C5+are the predominant products. In the presence of BEA catalysts, the product distribution in gas fractions is differentfrom that in the absence of catalyst. The main components in gas fractions from catalytic cracking are propene, n-butane, i-butene and C5+. Figure 7 shows carbon number distribution of distillate oil obtained by catalytic cracking.The major liquid products for all catalyst are distributed in the range of C7 to C9. That is comparable to distributionof distillate oil obtained in this work based on the boiling point rang using n-paraffin as a reference. In conclusion,the Si/Al ratio of 30 is a powerful catalyst and was selected for the study on the effect of reaction temperature.BEA with the Si/Al ratio of 30 was used as a catalyst for studying the influence of reaction temperature on itsactivity and the thermal cracking was tested in comparison. The values of %conversions and product distribution forthermal and catalytic cracking of PP waste at 350, 380, 400 and 420°C are shown in Table 3. The activities of thezeolite in term of %conversion are very high up to 96% in the temperature range from 380 to 420°C and aretemperature independent. Sakata et al. (1999) reported that thermal cracking of PP waste at 380oC shows a highamount of liquid and gas product. Below the temperature of 380°C the conversion is affected by the temperature.The distribution of both gas and liquid products are also affected by temperature when the temperature was loweredthan 380oC. For the temperature in the range of 380 to 420oC, the products are mainly in liquid fractions at the highyield about 51-53% with minor product in gas fractions at the yield about 42 to 44%. The results are similar toDemirbas (2000). The effect of BEA on PP waste cracking clearly can be observed at the residue of catalyticcracking which dramatically reduces from 78.8 to 4.5% compared with the thermal cracking. Figure 8 shows thedistribution of gas fractions provided by catalytic cracking. The major components for catalytic cracking arepropene, n-butane, i-butene and C5+. When the reaction temperature increases, lighter hydrocarbons (methane andethane) also increases. While the components of thermal cracking are C1 through C5, the major components arepropene and n-pentane (not shown). The growing yield of volatile components as function of temperature could becaused by the differences in the thermal stability of polymer chain because the hydrocarbon has reducing thermalstability with increasing temperature. Therefore, the C-C bonds were cracked more easily at 400 and 420oC than atlower temperature, and it resulted in higher yield of volatile products. Considering the gas selectivity of catalyticcracking of PP waste at 420oC, it was found that n-butane is lower and i-pentane is higher at 400oC due to the effectof thermal cracking with catalytic cracking. Figures 9 shows the carbon number distribution of distillate oil fromcatalytic cracking with different reaction temperatures. The distillate oil components are mainly in the range of C7 toC9 for reaction temperatures at 380 to 420oC while C8 and C9 are major products at 350oC. This result indicates thatthe liquid product distribution depends on the temperature only at low temperature. The conversion and productdistribution obtained at the temperatures of 380oC and 400oC are not different. For thermal cracking at 380oC, theliquid fraction is rich of C9. For the thermal cracking at 400 and 420oC, the liquid hydrocarbon fractions aredistributed in a wide range of equivalent hydrocarbons from C6 to C9 (not shown). It is well known that the thermalcracking occurs by random scissoring of the long polymeric chain, and the products of cracking are distributed in awide range of molecular weights. This result has been observed by Hwang et al. (2002), degradation of PP waste aredistributed in a narrow range of carbon number compared with thermal degradation.3.2.2 Activities of Regenerated BEA in PP Waste CrackingThe values of %conversion and %yield obtained by the PP waste cracking using fresh and regenerated BEA withSi/Al ratio of 30 catalysts at 380ºC are shown in Table 4. The values of %conversion are not different from freshcatalyst. The regenerated catalyst provides relatively lower yield of gas fraction and higher residue comparing to thefresh catalyst. Relatively more amount of residue, especially in form of wax remains in the reactor of theregenerated catalyst rather than that of fresh catalyst. This result suggests that the regenerated catalysts have lessspecific surface area and acidity than the fresh catalyst. The gas fraction composes the same product distribution.There is no difference in selectivity in gas fraction among the four catalysts. The product distributions of liquidfraction obtained by catalytic cracking of PP waste using the fresh and regenerated BEA provide mainly C7 and C8while C8 and C9 are mainly products for the third regenerated, indicating that the acidity of catalyst at the thirdregenerated is reduced by several calcinations before used.
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 2013364. ConclusionsThe nanoparticle BEA was successfully prepared by using a novel method. The Si/Al ratios were varied in a rangefrom 10 to 90. It is found that the Si/Al ratio as low as 10, the failure of formation of BEA is owing to amount oforganic template under the synthesis condition, acting as the skeleton for inorganic ions to adhere is not enough forall ions especially aluminum ionic species to form aluminosilicate building blocks. It is obvious that the Si/Al ratioof 30 provided with the sample with highest external surface area. BEA is found very active in cracking of PP wasteto liquid fuel. The thermal cracking of PP waste leads to plastic %conversion lower than catalytic cracking. Theplastic conversions and the yields of products fractions obviously depend on the reaction temperatures and Si/Alratios. It is interesting to note that the product selectivity is affected by those factors. In the catalytic cracking of PPwaste at 380oC over BEA (Si/Al = 30) is powerful catalyst shows greater %conversion than 95% due to the drasticinfluence of external surface area and acidity of the catalyst. The gas products obtained are mainly propene, i-buteneand C5+. The liquid products obtained by cracking of plastic are mainly in the boiling point ranging from C6 to C9.The used catalyst can be regenerated easily by calcination and its activity remains comparable to the fresh catalystAcknowledgementThailand-Japan Technology Transfer Project (TJTTP-JBIC), Chulalongkorn University is appreciated forcharacterization instruments and the 90th Anniversary of Chulalongkorn University Fund is thankful for financialsupport.ReferencesAchilias, D.S., & Megalokonomos, P. (2006). J. Environ. Prot. Ecol. 7, 407-413.Achilias, D.S., & Karayannidis, G.P. (2004). Water Air Soil Pollut. Focus. 4, 385-396.Aguado, J., Solelo, J. L., Serrano, D. P., Calles, J. A., & Escola, J. M. (1997). Energy & Fuels., 11, 1225.Aguado, J., Serrano, D. P., Escola, J. M., Garagorri, E., & Fernández, J. A. (2000). Polym. Degrad. Stab., 69, 11.Aguado, J., Serrano, D.P., Escola, J. M., & Peral, A. (2008). J. Anal. Appl. Pryrolysis. 85, 352-358.Artetxe, M., Lopez, G., Amutio, M., Elordi, G., Bilbao, J., & Olazar, M. (2012). Chem. Eng. J. 207-208, 27-34.Bregolato, M., Bolis, V., Busco, C., Ugliengo, P., Bordiga, S., Cavani, F., Ballarini, N., Maselli, L., Passeri, S., &Forni, L. (2007). J. Catal. 245, 285.Demirbus, A. (2000). J. Anal and Appl. Pyrolysis. 72, 97-102.Ding, L., Zheng, Y., Zhang, Z., Ring, Z., & Chen, J. (2006). Micropor. Mesopor. Mater. 94, 1.Hulea, V., & Dumitriu, E. (2004). Appl. Catal. A. 277, 99.Hwang, E. Y., Kim, J. R., & Choi, J. K. (2002). J. Anal. Appl. Pryrolysis. 62, 351-364.Isihara, Y., Nanbu, H., Saido, K., Ikemura, T., & Takesue, T. (1992). Polymer. 33, 3482.Jon, H., Nakahata, K., Lu, B., Oumi, Y., & Sano, T. (2006). Micropor. Mesopor. Mater. 94, 72.Kumar, N., Masloboischikova, O. V., Kustov, L. M., Hweikkila, T., Salmi, T., & Murzin, D. Y. (2007). Ultrason.Sonochem. 14, 122.Lee, K. H., Noh, N. S., & Valenci, S. (2002). Degradation and Stability. 78, 539-544.Lee, Y. J., Kim, J. H., Kim, S. H., Hong, S. B., & Seo, G. (2008). Appl. Catal. B. 83, 160.Manos, G., Yusof, T., Gangas, N.A., & Papayannakos, N. (2002). Energy Fuel. 16, 485-489.Nakao, R., Kubota, Y., Katada, N., Nishiyama, N., Kunimori, K., & Tomishige, K. (2004). Appl. Catal. A: General.273, 63.Obali, Z., Sezgi, N. A., & Dogu, T. (2012). Chem. Eng. J. 207-208, 421-425.Panda, A. K., & Singh, R. K. (2011). J. Fuel Chem. Techno. 39 (3), 198-202.Renzini, M. S., Lerici, L., Sedran, U., & Pierella, L. B. (2011). J. Anal. Appl. Pryrolysis. 92, 450-455.
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 201337Sakata, Y., Uddin, A., & Muto, A. (1999). J. Anal. Appl. Pyrolysis. 51, 135.Sakthivel, A., Iida, A., Komura, K., Sugi, Y., & Chary, K.V. R. (2009). Micropor. Mesopor. Mater. 119, 322.Scheirsr, J. (1998). Polymer Recycling. J. Wiley & sons, W. Sussex.Selvam, T., Bandarapu, B., Mabande, G. T. P., Toufar, H., & Schwieger, W. (2003). Micropor. Mesopor. Mater. 64,41.Seo, Y. H., lee, K. H., & Shin, D.H. (2003). J. Anal. Appl. Pryrolysis. 70, 383.Thailand Energy and Environment Network (TEENT), (2012), Turning Plastic Waste into Crude Oil. [online]Avaiable: http://teenet.tei.or.th/Knowledge/plastictooil.html (March 12, 2012).Wadlinger, R. L., Kerr, G. T. & Rosinski, E. J. (1967). US Pat 3,308,069.Xia, Q. H., & Tatsumi, T. (2005). Mater. Chem. Phys. 89, 89.Zhao, D., Feng, J., Hua, Q., Malosh, N., Fredrickson, G. H., Chmelka, B. F. & Stucky, G. D. (1998). Science. 279,548.Table 1: Transformation of SBA-15 into zeolite beta at various conditionsTable 2: Values of %conversion and %yield obtained from thermal cracking and catalytic cracking of PP wate overBEA with various Si/Al ratios.Silicasourceyield%Si/Alin gelSEMParticlesize (nm)BETSurfacearea (m2/g)Externalsurfacearea (m2/g)ProductphaseNH3-TPD acidity (mmol/g)weaker(170oC)stronger(200oC)totalTEOS - - 50 x 110 797 - SBA-15 n/a n/a n/aSBA-15 n/a 10 n/a 346 n/a amorphous n/a n/a n/aSBA-15 79.8 30 173 782 106.9 BEA 1.09 0.12 1.21SBA-15 71.8 60 215 781 43.4 BEA 0.71 0.23 0.94SBA-15 6.0 90 211 455 41.1 BEA 0.51 0.28 0.8%conversionThermal 350oC Si/Al = 30 Si/Al = 60 Si/Al = 902.0 50.5 42.9 44.2%yield1. gas fraction 2.0 33.1 27.5 27.32.liquid fraction - 17.4 15.4 16.9-% distillated oil - 85.0 82.5 77.5-% heavy oil - 15.0 17.5 22.53. residue 98.0 49.5 57.1 55.8
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 2013385 10 15 20 25 30 35 402-theta (degree)0.5 1.5 2.52-theta (degree)Intensity(a.u.)(b)(a)(d)(c)(d)(c)(b)(a)Table 3: Values of %conversion and %yield obtained by thermal cracking and catalytic cracking of PP waste atvarious temperaturesTable 4: Values of %conversion and %yield obtained by catalytic cracking of PP waste using the fresh and theregenerated catalysts.Figure 1: XRD patterns of calcined BEA with various Si/Al molar ratios: (a) 10, (b) 30, (c) 60 and (d) 90.%conversion350oC 380oC 400oC 420oCBEA thermal BEA thermal BEA thermal BEA thermal50.5 2.0 95.5 21.2 96.0 60.0 96.1 93.3%yield1. gas fraction 33.1 2.0 42.9 14.3 42.6 25.2 44.5 41.12.liquid fraction 17.4 - 52.6 6.9 53.4 34.8 51.5 52.2-%distillated oil 85.0 - 77.6 55.1 77.9 53.2 75.7 55.3- %heavy oil 15.0 - 22.4 44.9 22.1 46.8 24.3 44.63. residue 49.5 98.0 4.5 78.8 4.0 40.0 3.9 6.7%conversionFresh BEA 1stRegenerated 2ndRegenerated 3rdRegenerated95.8 95.1 93.5 85.6%yield1. gas fraction 42.2 40.5 37.7 36.62. liquid fraction 53.6 54.6 55.8 49.0- %distillate oil 39.0 39.8 42.2 36.8- %heavy oil 14.6 14.8 13.6 12.23. residue 4.2 4.8 6.5 14.4
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 20133901002003004005006007008000 0.2 0.4 0.6 0.8 1P/P0Va/cm3(STP)g-1SBA-15Si/Al = 10Si/Al = 30Si/Al = 60Si/Al = 90(a)(b)(c)200 150 100 50 0 -50 -100 ppmFigure 2: 27Al-MAS-NMR spectra of calcined BEA catalysts with different Si/Al ratios in catalyst (a) 30, (b) 60 and(c) 90.Figure 3: SEM images of calcined BEA with various Si/Al ratios of (a) 10, (b) 30, (c) 60 and (d) 90Figure 4: Nitrogen adsorption isotherms of calcined Products.a be.c.ba.d.
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 20134005101520253035MethaneEthaneEthenePropanePropenei-Butanen-Butanet-2-Butene1-Butenei-Butenecis-2-Butenei-Pentanen-PentaneMethylAcetyleneC5+%SelectivitySi/Al = 30Si/Al = 60Si/Al = 90thermal 350°C05101520253035C5 C6 C7 C8 C9 C10 C11 C12 C13 C14 C14+%SelectivitySi/Al = 30Si/Al = 60Si/Al = 90Figure 5: NH3-TPD profiles of BEA with various Si/Al ratios in catalyst of (a) 30, (b) 60 and (c) 90..Figure 6: Product distribution of gas fraction obtained by catalytic cracking of PP using BEA with various Si/Alratios.Figure 7: Carbon number distribution of liquid fraction from catalytic cracking over BEA with various Si/Al ratios.100 200 300 400 500 600Temperature (oC)Desordedamountofammonia(uVolt)(c)(b)(a)
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.4, 20134105101520253035MethaneEthaneEthenePropanePropenei-Butanen-Butanet-2-Butene1-Butenei-Butenecis-2-Butenei-Pentanen-PentaneMethylAcetyleneC5+%Selectivity350°C380°C400°C420°C0510152025303540C5 C6 C7 C8 C9 C10 C11 C12 C13 C14 C14+%Selectivity350°C380°C400°C420°CFigure 8: Product distribution of gas fraction obtained by catalytic cracking over BEA (Si/Al = 30) with variousreaction temperatures.Figure 9: Carbon number distribution of liquid fraction from catalytic cracking over BEA (Si/Al = 30) with variousreaction temperatures.
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgCALL FOR PAPERSThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. There’s no deadline forsubmission. Prospective authors of IISTE journals can find the submissioninstruction on the following page: http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar